Controllable Band Alignment Transition in InSe–MoS2Van der Waals Heterostructure
Xi Chen, Zheng-Zhe Lin,* and Ming Ju
Van der Waals (vdW) heterojunctions with type-II band alignment, in whichelectrons and holes are localized in distinct layers, play a central role inoptoelectronic devices and solar cells. The present study analyzes a type-I!IIband alignment transition in InSe–MoS2 vdW heterostructure, proposed to becontrolled via changing interlayer distance or applying perpendicular externalelectric field. The band position shift of InSe relative to that of MoS2attributes to a surface polarization mechanism. Changing band offset intotype II facilitates possible use and allows greater flexibility for bandengineering of InSe–MoS2 heterostructure in optoelectronic and solar energyapplications. The present findings provide theoretical guidance to a newapproach to improve the optoelectronic properties of vdW heterostructures.
The birth of two-dimensional materials launched a greatrevolution in material science. Several two-dimensional materi-als have been considered as building blocks for future nano-electronics and optoelectronics. They can lead to drasticreduction in characteristic lengths of electronic devices.[1–3] Asisolated atomic planes, two-dimensional materials can bereassembled by designing layered heterostructures, which areoften called van der Waals (vdW) heterostructures.[4–6] Withdistinctive electronic and optoelectronic properties,[7–11] vdWheterostructures have awakened many research efforts for theirpotential applications in light-emitting diodes, solar cells, andhigh-electron-mobility transistors. At present, vdW heterostruc-tures built by graphene,[12–14] phosphorene, and transition-metal dichalcogenides (TMDs)[16–18] have been studied inexperiments and theory. A strong photoinduced modulationdoping effects in graphene-BN vdW heterostructures werefound. As building blocks, different two-dimensional materi-als can assemble various vdW heterostructures, revealing newphysical properties and phenomena.
Dr. X. Chen, Prof. Z. -Z. LinSchool of Physics and Optoelectronic EngineeringXidian UniversityXi’an 710071, P.R. ChinaE-mail: [email protected]
Dr. M. JuSchool of Economics and ManagementShanghai Technical Institute of Electronics and InformationShanghai 200018-201411, P.R. China
The ORCID identification number(s) for the author(s) of this articlecan be found under https://doi.org/10.1002/pssr.201800102.
The band alignment of vdW heterostruc-tures is crucial in applications of optoelec-tronics. Several experimental investigationshave shown that underlying type-II bandalignment is required for optoelectronicsand solar cell applications.[16,20,21] For two-dimensional vdW heterostructures withtype-II band alignment, electrons and holesare spatially separated in distinct layers andform interlayer excitons, thus electron-holerecombination could be avoided. Suchspatial charge separation leads to longelectron-hole recombination lifetime[22,23]
and plays a central role in the internalprocess of solar cells. If the bandalignment can be controlled and switchedto type-II, more vdW heterostructures are
then suitable for optoelectronic and solar energy applications.In recent years, research efforts have been centered upon
devices based on two-dimensional semiconductors such asTMDs and black phosphorene attributed to their exoticproperties.[25–27] Recently, indium selenide (InSe) whichbelongs to III-VI layered semiconductor family has beensuccessfully prepared. On the one hand, Single-layer InSeexhibits high carrier mobility up to 103 cm2V�1 s�1,[30,31] highon-off current ratio (�103), and large broadband spectralresponse. Considered as key elements for optoelectronic andnanoelectronic applications attributed to its novel properties,InSe has attracted great interest.[30,33–36] On the other hand,two-dimensional TMDs have also proved promising funda-mental building blocks for ultrathin high-performance devi-ces.[37–39] Research works have demonstrated and predicted thatTMD field-effect transistors show high on/off current ratio(104� 108) with less short-channel effects. Considering InSe–MoS2 heterostructure has been grown by molecular beamepitaxy, the band engineering in InSe–MoS2 vdW hetero-structure is worth studying.
The goal of this paper is to investigate the band structure andproperties of two-dimensional InSe–MoS2 vdW heterostructurebased on density functional theory (DFT) calculations. The InSe–MoS2 heterostructure presents a type-I!II band alignmenttransition, controlled by changing interlayer distance. The bandposition shift of InSe relative to that of MoS2 attributes to asurface polarization mechanism. Moreover, it is showed that thetype-I!II band alignment transition can be also realized by theapplication of perpendicular external electric field. This allowsmanipulation of the band properties and flexibility for bandengineering of InSe–MoS2 heterostructure in optoelectronic andsolar energy applications. The present results are essential to thedesign of future nanoelectronic and optoelectronic devices and
propose a new approach to improve the properties of two-dimensional vdW heterostructures.
Computational Methods: In the simulation model, 3� 3 InSemonolayer is matched to 4� 4 MoS2 monolayer. The latticeconstant mismatch is less than 2%. Periodic boundaryconditions are applied. To avoid the interactions betweennearest slabs, the replicas of simulation systems are separatedby a large spacing of 30 A along the z direction (perpendicular tothe two-dimensional surface).
First-principles calculations are performed within spin-polarized DFT by using Vienna ab initio simulation package(VASP). Projector-augmented wave (PAW) method is usedto account electron-ion interactions. In all the calculations, aplane-wave basis set with kinetic energy cutoff of 400 eV is usedto expand the wave functions. The convergence of the totalenergy was considered to be achieved until two iterated stepswith energy difference less than 10�5 eV. The Brillouin zone issampled by using 3� 3� 1 Γ-centered Monkhorst–Pack grid. AGaussian smearing with a width of σ¼ 0.05 eV is used.
In geometry optimizations and total energy calculations, theoptB88-vdW dispersion-corrected exchange functional,[43,44]
which has been demonstrated as a reliable approach to describedispersive forces in 2D systems, is employed to correctlydescribe the effect of a vdW interaction. Geometry optimizationsare performed until the Hellmann–Feynman forces acting oneach atom are less than 0.01 eV A�1. Ground state structures arefound by using the conjugate gradient method.
To account for the band gaps and band edge positions, theHeyd–Scuseria–Ernzerhof (HSE06) hybrid functional[46,47] isused to calculate the band structures of the optimized systems.In general, HSE06 hybrid functional provides more accurateband gaps as well as band alignment. The band structures andabsolute band energies are aligned with respect to the vacuumlevel obtained via electrostatic potential.
Basic properties and band alignment: The InSe monolayerlattice (Figure 1a) has hexagonal symmetry, with a thickness offour atoms linked in the Se─In─In─Se sequence via covalent
Figure 1. Basic properties of InSe monolayer. a) Top and side view of InSemonolayer. b) Band structure of InSemonolayer at the level of HSE06. Redand blue lines denote the calculation results with and without SOC,respectively. The Fermi level is shown by dashed line. The energy ofvacuum level is set zero.
Phys. Status Solidi RRL 2018, 12, 1800102 1800102 (
bonds with the In atoms at tetrahedral sites. The rhombic unitcell is shown by dashed lines in Figure 1a. The calculated latticeconstant a¼ 4.09 A is in agreement with previous experimen-tal[28,48] and theoretical[28,49,50] results. In InSe monolayer, anindirect band gap (shown by the arrow in Figure 1b is observed,with the conduction band minimum (CBM) at the Γ point andthe valence band maximum (VBM) lying between the Γ and Kpoints. The spin-orbit coupling (SOC) induces a splitting ofsome bands (see red lines in Figure 1b by about 0.1 eV (as seen,e.g., at K, Γ, and M points). Generally, hybrid HSE06 functionalprovides more accurate band gap than standard DFT approach.Ideally, one should also employ GWmany-body theory to obtainreliable band energies. (It is worth noting that the vertexcorrection, which is ignored by the GW method, is veryimportant for the band alignment. Recent report indicates thatthe vertex mainly shifts the bands of two-dimensional semi-conductors relative to vacuum by 0.5 eV.) Here, the Perdew–Burk–Ernzerhof (PBE) functional, HSE06 functional and GW0calculations (starting from HSE06 orbitals) are performed forInSe single cells to obtain band gap.With the PBE functional, thecalculated band gap is 1.42 (1.39) eV with (without) SOC,respectively. With the HSE06 functional, the calculated band gapis 2.15 (2.12) eV with (without) SOC, respectively. The GW0calculation further increases the band gap. With GW0calculation, the calculated band gap is 2.96 (2.93) eV with(without) SOC, respectively (in agreement with Debbichiet al.). The differences between PBE, HSE06 and GW0calculations are mostly a shift of band structure. The GW0calculation provides more accurate band gap, but takes muchmore computation time. So, in the following text, HSE06functional is employed without SOC for all the calculations.
Before investigating the properties of InSe–MoS2 hetero-structure, we first understand the band alignment of InSe andMoS2 monolayers. DFT calculations suggest a band alignmenttransition in the combination of InSe andMoS2 monolayers. Forisolated InSe and MoS2 monolayers, the band structures arepredicted to be type-II band alignment (Figure 2a), i.e., the VBMof MoS2 is higher than the VBM of InSe
ΔVB ¼ EVBMMoS2 � EVBM
InSe > 0� �
; and meanwhile, the CBM of
MoS2 is higher than the CBM of InSe
ΔCB ¼ ECBMMoS2 � ECBM
InSe > 0� �
: When the InSe and MoS2
Figure 2. Band alignment of InSe and MoS2. a) Isolated and combinedInSe and MoS2 monolayers. b) Calculated band alignment of separatedInSe and MoS2 monolayers at the level of PBE, HSE06 and GW0. Theenergy of vacuum level is set zero.
monolayers constitute vdW heterostructure, the band alignmentchanges into type-I (Figure 2a), i.e.,ΔVB ¼ EVBM
MoS2 � EVBMInSe < 0
and ΔCB ¼ ECBMMoS2 � ECBM
InSe > 0: To verify the reliability of ourcalculations, the band structures of isolated InSe and MoS2monolayers are calculated by using PBE, HSE06 and GW0calculations (Figure 2b). The PBE calculation provides band offsetΔVB ¼ EVBM
MoS2 � EVBMInSe ¼ 0:04 eV and ΔCB ¼ ECBM
MoS2 �ECBMInSe ¼ 0:03 eV:However, the PBE resultmay be quantitatively
inaccurate, while the HSE06 and GW0 results are more reliable.
Figure 3. The band structure and alignment of InSe–MoS2 heterojunction chvdW heterostructure. Periodic boundary is shown by dashed lines. b) Projecteinterlayer distance d¼ 3.3, 4.3, 6.3, and1 A. The green projection comes fromshown by dashed lines. The energy of vacuum level is set zero. c) The banddistance d. d) Isosurfaces of charge redistribution with values of �10�4 e A
Phys. Status Solidi RRL 2018, 12, 1800102 1800102 (
TheHSE06 calculation providesΔVB¼ 0.13 eVandΔCB¼ 0.11 eV.The GW0 calculation provides larger band gaps than HSE06, andthe GW0-predicted band offset ΔVB¼ 0.14 eV and ΔCB¼ 0.12 eVare similar to HSE06. Although HSE06 still underestimates theband gaps relative to GW0 by 0.81 eV for InSe and 0.81 eV forMoS2, theHSE06 is significantly closer to theGW0 result than thePBE. Therefore, HSE06 functional is used throughout the paperfor band offset calculations.
Band alignment control via interlayer distance control: In thissection, we study controlling the band alignment of InSe–MoS2
anging with interlayer distance. a) The top and side views of InSe–MoS2d band structure of InSe–MoS2 heterostructure at the level of HSE06 withthe InSe layer and the blue comes from the MoS2 layer. The Fermi level isgap (upper) and band offset (lower) varying with enlarging InSe–MoS2
Figure 4. Energetics of InSe–MoS2 heterostructure. The change of InSe–MoS2 binding energy Ub with interlayer distance d.
heterostructure via changing the interlayer distance. Thesimulation model of InSe–MoS2 vdW heterostructure is setup by matching 3� 3 InSe monolayer to 4� 4 MoS2 monolayer(Figure 3a), with a supercell lattice constant of 12.50 A. Thelattice constant mismatch of InSe (MoS2) is þ1.8 (�1.9)%,respectively. In the most stable structure, the vertical distancefrom the bottom of MoS2 layer to the top of InSe layer is 3.3 A(Figure 3a). Such distance is larger than the sum of the covalentradii of S and Se atoms, indicating no chemical bonds at theInSe–MoS2 interface.
Before studying the effect of interlayer distance, we firstinvestigate band properties of the most stable structure of InSe–MoS2 heterostructure. The 1st of Figure 3b plots the projectedband structure of the most stable InSe–MoS2 heterostructure,with interlayer distance d¼ 3.3 A. The green projection comesfrom the InSe layer and the blue comes from theMoS2 layer. Theelectronic states of the InSe and the MoS2 layers are weaklyperturbed upon the formation of InSe–MoS2 heterostructure.We found that the band gap of InSe/MoS2 change by less than0.13/0.01 eV, respectively. In the 1st panel of Figure 3b, the InSe–MoS2 heterostructure presents a type-I band alignment with avalence band offset ΔVB ¼ EVBM
MoS2 � EVBMInSe ¼ � 0:10 eV and a
conduction band offset ΔCB ¼ ECBMMoS2 � ECBM
InSe ¼ 0:62 eV:Next, we gradually enlarge the interlayer distance d and
observe the change of band structure. The lower panel ofFigure 3c plots ΔVB and ΔCB varying with enlarging InSe–MoS2distance d. In the range of d¼ 4� 5 A, the band alignment ofInSe–MoS2 heterostructure changes from type-I (ΔVB< 0 andΔCB> 0) to type-II (ΔVB> 0 and ΔCB> 0). In the 2nd panel ofFigure 3b, the band structure of InSe–MoS2 heterostructure withd¼ 4.4 A is depicted, presenting a type-II band alignment withΔVB¼ 0.13 eV and ΔCB¼ 0.70 eV. The InSe–MoS2 heterostruc-ture presents a semiconducting character with an indirect bandgap of 1.68 eV, with VBM at the K point and CBM lying at the Γpoint. In the projected band structure of Figure 3b, we can seethat VBM lies on the InSe layer while CBM is localized in theMoS2 layer, which is suitable in order to promote the electron-hole separation. With enlarging interlayer distance d> 4.4 A, theband structure of InSe–MoS2 heterostructure only has a littlechange. The 3rd panel of Figure 3b depicts the band structure ofd¼ 6.3 A, presenting a type-II band alignment with ΔVB¼ 0.16eV and ΔCB¼ 0.73 eV which are almost equivalent to those ofisolated InSe and MoS2 layers (the 4th panel of Figure 3b).
In terms of change of interlayer distance d, the band gapslightly changes with it. The upper panel of Figure 3c plots theband gap of InSe and MoS2, and the band gap of InSe–MoS2heterostructure. In the range of d¼ 3.3� 9.3 A, the band gap ofMoS2 seldom changes, while the band gap of InSe slightlyincreases. In the change of d, the band gap of InSe–MoS2heterostructure changes a little, from 1.68 to 1.66 eV. Accordingto results above, the change of interlayer distance d only affectsband alignment of InSe–MoS2 heterostructure but seldomchanges band gap. This characteristic is beneficial for the use ofInSe–MoS2 heterostructure as adjustable device, with flexiblecontrol of band alignment and without changing band gap.
To gainmore insight into the change of band alignment,we payattention to the interactionandchargeredistributionbetweenInSeandMoS2 layers.As the InSe andMoS2 layershavedifferentFermi
Phys. Status Solidi RRL 2018, 12, 1800102 1800102 (
energy, electrons would slightly redistribute when the two layersget close to each other, leading to the rise/drop of InSe/MoS2valance band. To visualize the charge redistribution, we plot theisosurface of charge redistribution in the InSe–MoS2 hetero-structure for the case of d¼ 3.3 A in Figure 3d. It can be seen thatslight charge redistributionhappensmainly in the region betweenthe InSe and MoS2 layers. In the InSe layer, the electrons arerepulsed by the MoS2 layer, showing more negative charge areanear the centers of Se atoms. Such repulsion leads to theenhancement of InSe valence band. On the contrary, in the MoS2layer the electrons are attracted by the InSe layer, showing morenegative charge area in the region between the InSe and MoS2layers. Such electronic attraction onMoS2 leads to the reduction ofMoS2 valence band. The electron redistribution reveals apolarization near InSe–MoS2 contact surface that causes theslight interaction between InSe and MoS2 layers.
In addition, the stability of InSe–MoS2 heterostructure isexamined by comparing the total energies of relaxed InSe–MoS2system UInSe�MoS2ð Þ with ones of isolated InSe and MoS2 layersUInSe and UMoS2ð Þ: The UInSe and UMoS2 are obtained byconsidering the strained 3� 3 InSe and 4� 4MoS2 supercells.
The binding potential is calculated as Ub ¼ UInSe�MoS2 �ðUInSe þ UMoS2Þ ¼ � 18:9meV A�2
; which is lower thanthe binding potential of InSe-phosphorene heterostructure(�9.03meV A�2. The stability of InSe–MoS2 heterostructureis further revealed by the change of interlayer binding energy.Starting from interlayer balance distance d¼ 3.3 A, interlayerbinding energy Ub decreases with enlarging d (Figure 4). In therange of d¼ 3.3� 5.0 A, Ub¼�18.9��8.93meV A�2 keepslower than the binding potential of InSe-phosphorene hetero-structure. In this range of d, InSe–MoS2 heterostructure keepsmore stable than InSe-phosphorene heterostructure. Whenmanipulating the band alignment via changing interlayer
distance in this range, the stability of InSe–MoS2 heterostructurecould be guaranteed.
Band alignment control via external electric field: In this section,we further consider controlling the the band alignment viaapplying external electric field. For InSe–MoS2 heterostructure inthe equilibrium interlayer distance d¼ 3.3 A (type-I bandalignment, ΔVB ¼ EVBM
MoS2 � EVBMInSe < 0), an external electric
field pointing fromMoS2 to InSe is applied. Then, electrons driftfrom InSe to MoS2 and the band alignment would change fromtype-I to type-II. Figure 5a plots the projected band structure withperpendicular external field e¼ 0, 0.2, and 0.4 eV A�1. It can beseen that the band of InSe graduallymoves down relative to that ofMoS2 with increasing electric field, leading to enlarging ΔVB andΔCB. For e> 0.2 eV A�1, the band alignment is changed o type-II
ΔVB ¼ EVBMMoS2 � EVBM
InSe < 0� �
: The lower panel of
Figure 5b plots the change of ΔVB and ΔCB along with externalelectric field e¼�0.2� 0.4 eV A�1. The result above offers us asimple way to control the band alignment by applying bias voltageon the InSe–MoS2 heterostructure. For d¼ 3.3 A, a voltage of0� 2Vcangenerateanelectricfieldofabout0�0.6V A�1,which islarge enough for the band offset control.We then performdetailedcalculations for external field e¼�0.2� 0.4 eV A�1, and findlinear relation of band gap dependent on e (Figure 5b).
Conclusion: In conclusion, the InSe–MoS2 heterostructurepossesses well-controlled interfacial electronic properties andband structure which could be manipulated by changing
Figure 5. The band structure and alignment of InSe–MoS2 heterojunction chaheterostructure at the level of HSE06 with interlayer distance d¼ 3.3 A, andshown by dashed line. b) The band gap (upper) and band offset (lower) va
Phys. Status Solidi RRL 2018, 12, 1800102 1800102 (
interlayer distance or applying external electric field. DFTcalculations reveal the stability of two-dimensional InSe–MoS2vdW heterostructure. It is evident that there are no chemicalbonds at the InSe–MoS2 interface. The electronic states of InSeand MoS2 layers are mostly preserved upon the formation ofInSe–MoS2 heterostructure, and nearly independent of paralleldisplacement of MoS2 on InSe. An intrinsic change from type-Ito type II band alignment occurs with enlarging interlayerdistance. The shift of the band position of InSe relative to thatof MoS2 attributes to a surface polarization mechanism,leading to slight electron redistribution between the InSe andMoS2 layers. Moreover, it is also possible to invoke the type-I!II band alignment transition by applying perpendicularexternal electric field or bias voltage. Overall, changing bandoffset to type II leads to possible use of InSe–MoS2heterostructure in optoelectronic and solar energy applica-tions. Our research proposes a new perspective on advantagenanoelectronic and optoelectronic devices with well-controlledfeature of vdW heterostructures, and also provides theoreticalguidance on improving the optoelectronic properties of vdWheterostructures.
AcknowledgementsThis work was financially supported by the Fundamental ResearchFunds for the Central Universities (No. JB180513) and the 111 Project(No. B17035).
nging with external electric field. a) Projected band structure of InSe–MoS2perpendicular external field e¼ 0, 0.2 and 0.4 eV A�1. The Fermi level isrying with external electric field.
Conflict of InterestThe authors declare no conflict of interest.
Keywordscontrollable band alignment, type-I!II transition, two-dimensional vander Waals heterojunctions
Received: March 6, 2018Revised: April 8, 2018
Published online: April 18, 2018
 S. Z. Butler, S. M. Hollen, L. Cao, Y. Cui, J. A. Gupta, H. R. Gutierrez,T. F. Heinz, S. S. Hong, J. Huang, A. F. Ismach, E. Johnston-Halperin,M. Kuno, V. V. Plashnitsa, R. D. Robinson, R. S. Ruoff, S. Salahuddin,J. Shan, L. Shi, M. G. Spencer, M. Terrones, W. Windl,J. E. Goldberger, ACS Nano 2013, 7, 2898.
 J. M. Hamm, O. Hess, Science 2013, 340, 1298. K. J. Koski, Y. Cui, ACS Nano 2013, 7, 3739. L. Britnell, R. V. Gorbachev, R. Jalil, B. D. Belle, F. Schedin,
A. Mishchenko, T. Georgiou, M. I. Katsnelson, L. Eaves,S. V. Morozov, N. M. R. Peres, J. Leist, A. K. Geim,K. S. Novoselov, L. A. Ponomarenko, Science 2012, 335, 947.
 A. K. Geim, I. V. Grigorieva, Nature 2013, 499, 419. R. Balu, X. L. Zhong, R. Pandey, S. P. Karna, Appl. Phys. Lett. 2012,
100, 1530. H.-P. Komsa, A. V. Krasheninnikov, Phys. Rev. B 2013, 88, 085318. W. Li, T. Wang, X. Dai, X. Wang, C. Zhai, Y. Ma, S. Chang, Solid State
Commun. 2016, 225, 32. X. Liu, Z. Li, J. Phys. Chem. Lett. 2015, 6, 3269.
 A. Ramasubramaniam,D.Naveh, E. Towe, Phys. Rev. B 2011, 84, 3239. C. Tan, Q. Yang, R. Meng, Q. Liang, J. Jiang, X. Sun, H. Ye, X. P. Chen,
J. Mat. Chem. C 2016, 4, 8171. W. Li, T.-X. Wang, X.-Q. Dai, X.-L. Wang, Y.-Q. Ma, S.-S. Chang, Y.-
N. Tang, Physica E 2017, 88, 6. J. E. Padilha, A. Fazzio, A. J. R. da Silva,Phys. Rev. Lett. 2015, 114, 066803. F. Zhang, W. Li, X. Dai, Superlattices Microstruct. 2016, 100, 826. L. Huang, J. Li, Appl. Phys. Lett. 2016, 108, 147. H. Fang, C. Battaglia, C. Carraro, S. Nemsak, B. Ozdol, J. S. Kang,
H. A. Bechtel, S. B. Desai, F. Kronast, A. A. Unal, G. Conti, C. Conlon,G. K. Palsson, M. C. Martin, A. M. Minor, C. S. Fadley,E. Yablonovitch, R. Maboudian, A. Javey, Proc. Natl. Acad. Sci.USA 2014, 111, 6198.
 Y. Ma, X. Zhao, T. Wang, W. Li, X. Wang, S. Chang, Y. Li, M. Zhao,X. Dai, Phys. Chem. Chem. Phys. 2016, 18, 28466.
 S. Latini, K. T.Winther, T.Olsen, K. S. Thygesen,NanoLett.2017,17, 938. L. Jun, J. Velasco, Jr., E. Huang, S. Kahn, C. Nosiglia, H.-Z. Tsai,
W. Yang, T. Taniguchi, K. Watanabe, Y. Zhang, G. Zhang,M. Crommie, A. Zettl, F. Wang, Nature Nanotechnol. 2014, 9, 348.
 H. Heo, J. H. Sung, S. Cha, B.-G. Jang, J.-Y. Kim, G. Jin, D. Lee, J.-H. Ahn, M.-J. Lee, J. H. Shim, H. Choi, M.-H. Jo, Nature Commun.2015, 6, 7372.
 P. Rivera, K. L. Seyler, H. Yu, J. R. Schaibley, J. Yan, D. G. Mandrus,W. Yao, X. Xu, Science 2016, 351, 688.
 M. Palummo,M. Bernardi, J. C. Grossman,Nano Lett. 2015, 15, 2794.
Phys. Status Solidi RRL 2018, 12, 1800102 1800102 (
 P. Rivera, J. R. Schaibley, A. M. Jones, J. S. Ross, S. Wu, G. Aivazian,P. Klement, K. Seyler, G. Clark, N. J. Ghimire, J. Yan, D. G. Mandrus,W. Yao, X. Xu, Nature Commun. 2015, 6, 6242.
 C.-H. Lee, G.-H. Lee, A. M. van der Zande, W. Chen, Y. Li, M. Han,X. Cui, G. Arefe, C. Nuckolls, T. F. Heinz, J. Guo, J. Hone, P. Kim,Nature Nanotechnol. 2014, 9, 676.
 Q. H. Wang, K. Kalantarzadeh, A. Kis, J. N. Coleman, M. S. Strano,Nature Nanotechnol. 2012, 7, 699.
 R. R. Q. Freitas, R. Rivelino, F. D. B. Mota, C. M. C. D. Castilho,A. Kakanakova-Georgieva, G. K. Gueorguiev, J. Phys. Chem. C 2016,119, 23599.
 R. R. Freitas, B. M. F. De, R. Rivelino, C. M. de Castilho,A. Kakanakova-Georgieva, G. K. Gueorguiev, Nanotechnology 2016,27, 055704.
 L.Debbichi, O. Eriksson, S. Leb�egue, J. Phys. Chem. Lett. 2015, 6, 3098. D. A. Bandurin, A. V. Tyurnina, G. L. Yu, A. Mishchenko, V. Z�olyomi,
S. V. Morozov, R. K. Kumar, R. V. Gorbachev, Z. R. Kudrynskyi,S. Pezzini, Nature Nanotechnol. 2017, 12, 223.
 S. Sucharitakul, N. J. Goble, U. R. Kumar, R. Sankar, Z. A. Bogorad,F. C. Chou, Y. T. Chen, X. P. A. Gao, Nano Lett. 2015, 15, 3815.
 W. Feng, W. Zheng, W. Cao, P. A. Hu, Adv. Mater. 2014, 26, 6587. S. R. Tamalampudi, Y. Y. Lu, U. R. Kumar, R. Sankar, C. D. Liao,
B. K. Moorthy, C. H. Cheng, F. C. Chou, Y. T. Chen, Nano Lett. 2014,14, 2800.
 S. Lei, F. Wen, L. Ge, S. Najmaei, A. George, Y. Gong, W. Gao, Z. Jin,B. Li, J. Lou, Nano Lett. 2015, 15, 3048.
 W. Feng, W. Zheng, X. S. Chen, G. Liu, P. A. Hu, ACS Appl. Mater.Interfaces 2015, 7, 26691.
 H. Jin, J. Li, L. Wan, Y. Dai, Y. Wei, H. Guo, 2D Mater. 2017, 4,025116.
 J. E. Padilha, R. H. Miwa, A. J. R. D. Silva, A. Fazzio, Phys. Rev. B 2017,95, 195143.
 O. Lopezsanchez, D. Lembke, M. Kayci, A. Radenovic, A. Kis, NatureNanotechnol. 2013, 8, 497.
 M. Massicotte, P. Schmidt, F. Vialla, K. G. Schädler,A. Reserbatplantey, K. Watanabe, T. Taniguchi, K. J. Tielrooij,F. H. L. Koppens, Nature Nanotechnol. 2016, 11, 42.
 A. Steinhoff, J.H.Kim,F. Jahnke,M.Rösner,D. S. Kim,C. Lee,G.H.Han,M. S. Jeong, T. O. Wehling, C. Gies, Nano Lett. 2015, 15, 6841.
 T. Hayashi, K. Ueno, K. Saiki, A. Koma, J. Cryst. Growth 2000, 219, 115. G. Kresse, J. Hafner, Phys. Rev. B 1993, 48, 13115. P. E. Blöchl, Phys. Rev. B 1994, 50, 17953. J. Klime�s, D. R. Bowler, A. Michaelides, J. Phys.: Condens. Matter
2010, 22, 022201. J. Klimes, D. R. Bowler, A. Michaelides, Phys. Rev. B 2011, 83, 772. H. Y. Guo, N. Lu, J. Dai, X. J. Wu, X. C. Zeng, J. Phys. Chem. C 2014,
118, 14051. J. Heyd, G. E. Scuseria, M. Ernzerhof, J. Chem. Phys. 2003, 118, 8207. J. Heyd, G. E. Scuseria, M. Ernzerhof, J. Chem. Phys. 2006, 124,
219906. A. Politano, D. Campi, M. Cattelan, I. Ben Amara, S. Jaziri,
A. Mazzotti, A. Barinov, B. Gurbulak, S. Duman, S. Agnoli,L. S. Caputi, G. Granozzi, A. Cupolillo, Sci. Rep. 2017, 7, 3445.
 H. Jin, J. W. Li, Y. Dai, Y. D. Wei, Phys. Chem. Chem. Phys. 2017, 19,4855.
 H. Jin, J. W. Li, L. H. Wan, Y. Dai, Y. D. Wei, H. Guo, 2DMater. 2017,4, 025116.
 P. S. Schmidt, C. E. Patrick, K. S. Thygesen, Phys. Rev. B 2017, 96,205206.